Prevention of Hydrogen Embrittlement in Steels
H. K. D. H. Bhadeshiaa
aMaterials Science and Metallurgy, University of Cambridge, U.K
The essential facts about the nature of the hydrogen embrittlement of steelshave now been known for 140 years. It is diffusible hydrogen that is harmfulto the toughness of iron. It follows, therefore, that the harmful influence ofdiffusible hydrogen can be mitigated by preventing its entry into steel or byrendering it immobile once it penetrates the material. This review deals withthe methods that might be implemented to design steels and componentsthat resist hydrogen embrittlement by reducing the intake of hydrogen orrendering it innocuous when it does penetrate the steel.
Keywords: hydrogen embrittlement, hydrogen trapping, hydrogenpermeation, steel design, diffusion barriers, coatings
In the year 1875, Johnson  revealed extraordinary changes in the tough-ness and breaking-strain of iron that was immersed temporarily in acid forjust a few minutes. He further observed that the change is not permanentsince “with the lapse of time, the metal slowly regains it original toughnessand strength”. Indeed, he went on to observe that the moistened fracture sur-face of an embrittled steel liberated gas bubbles (“frothing”, with the bubbleseven seen under oil). The same paper found that a strong steel has a greaterloss in toughness due to immersion in acid than one which is soft. A numberof acids were studied and only those that produce hydrogen by their actionon iron were found to lead to a deterioration of properties. Furthermore, thehydrogen had to be nascent, not molecular, since leaving it in hydrogen gasdid nothing to the properties of the steel. To separate out the effect of acidand hydrogen, he designed an electrochemical charging method using only
Preprint submitted to January 18, 2016
Manchester town’s water, and proved that the iron electrode where hydrogenis liberated embrittled whereas the other one did not.
The paper by Johnson is a wonderful example of proper scientific method,which with elegantly simple experiments captured the essence of the embrit-tlement phenomenon, many aspects of which are rediscovered with muchfanfare in modern literature. The following conclusions can justifiably bereached from this 1875 paper:
1. it is hydrogen that embrittles steel, not the acid;
2. that the hydrogen is nascent, not molecular;
3. it is diffusible hydrogen that embrittles1, so the phenomenon is re-versible;
4. the effusion of diffusible hydrogen from the steel leads to frothing (bub-bles);
5. that stronger steel is more susceptible to embrittlement than softerversions.
The role of nascent hydrogen became well-established in the fifty yearsthat followed, and unique experiments were published to relate the embrit-tlement to microstructure. For example, Pfeil  showed that large-grainedsamples are more sensitive to hydrogen than those with fine structures. Hepostulated that hydrogen decreases the cohesion across cubic cleavage planes,but does not affect slip. Single crystals of iron were shown to be embrittledby hydrogen, an effect attributed to machining strains. The details of Pfeil’sand other contemporary work regarding cohesion or slip might be challengedin the light of modern understanding, but the 38,000 papers published sub-sequently on hydrogen embrittlement do not change the conclusions sum-marised above. One important phenomenon that emerged from diffusion
1The fact that diffusible hydrogen embrittles is now widely recognised and forms thebasis of many designs where the transport of hydrogen through the steel is impeded byintroducing traps [2–5, e.g.]. Hydrogen is present in minute quantities in steel, usually lessthan 1 part per million, but is attracted towards stress fields of the type associated witha crack tip. It therefore diffuses there, concentrates and thereby alters the fracture mech-anism to the detriment of steel. Hence the need for diffusible hydrogen for embrittlement.
measurements, is that diffusible hydrogen can be trapped at sites such asboundaries .2 That which is likely to be sufficiently strongly trapped maynot harm the steel. It follows that to produce steels that are resistant tohydrogen, all that is necessary is to control diffusible hydrogen. This canbe done by introducing benign traps in the steel or preventing the ingressof hydrogen. What follows below is based on this simple logic. We beginby considering methods that hinder the penetration of hydrogen into steels.Some of the coatings involved have multiple purposes, for example, aestheticappearance, retention of lubricant, etc. but at the same time are significantbarriers to hydrogen ingress.
2. Black Oxide
The so-called black oxide conversion-coating is generated on steel by im-mersion in an aqueous solution of 60-80% sodium hydroxide containing anoxidising agent such as 15-40% sodium or potassium nitrite or nitrate at atemperature of about 130-150 ◦C, for ≈ 30mins [9–11]. The final oxide ismagnetite , resulting from the following reaction sequence :
Fe2+ + 2H2O ! Fe(OH)2 + 2H+
Fe(OH)2 +OH−! Fe(OH)3
Fe(OH)3 +OH−! FeO−
2 + 2H2O
Fe2+ + 2FeO−
2 → Fe3O4 (1)
The oxide can also be a mixture of Fe3O4 and Fe2O3. The alkaline nature ofthe solution is important because there is no hydrogen evolved in the process(equation 1) which might otherwise embrittle the steel . The originalgoal of the black oxide coating was to provide some resistance to atmosphericcorrosion and this function can be enhanced by immersion of the componentin hot oil because the thin oxide film, typically 1-3µm, can otherwise bepermeable3. The coating does not compromise the friction coefficient andhence can be used for components such as bearings, although the benefits
2Pressouyre has suggested that even those features that repel hydrogen should hinderits progress through the lattice .
3It is argued in turn, that the presence of black oxide can improve the adhesion of thelubricant to the surface .
are not sustained under severe operating conditions [14, 15]. In many cases,black oxide coatings are introduced to enhance the aesthetic appearance ofthe product .
Black oxide has been applied to wind turbine bearings in an attempt toreduce the occurrence of axial cracks . One interpretation is that theoxide retards the diffusion hydrogen into the steel. Permeation4 experimentson pure iron on which a passive oxide film was produced using an equivolumemixture of 0.15NNa2B4O7 · 10H2O and 0.15NNH3BO3 on the anodic side ofa Devnathan and Stachurski cell, indicated a much lower influx of hydrogeninto iron that is coated . The film studied was only 2-3 nm thick, somethree orders of magnitude thinner than the black oxide coatings discussedhere. Such a thin film is unlikely to be representative in the context ofthe porosity that is known to exist in black oxide coatings. The detailedcomposition of the film was not stated in the original study. Nevertheless,the indications are that the diffusivity of hydrogen (DH) in the thin oxidefilm is some twelve orders of magnitude slower than in the pure, annealediron . There are no similar data for the thick black oxide films. However,when steel samples are stressed using a C-ring , it is claimed that thosethat are black-oxide coated and immersed in a corrosive solution fail laterthan uncoated controls; the evidence presented in support of this claim is at best regarded as schematic5. Nevertheless, there is a general impressionin the industry that oxides of metals including steel, reduce the permeabilityof hydrogen and its isotopes by at least an order of magnitude [20–22].
There may be additional factors that determine the utility of such ox-ide coatings. The coating may, for example, help reduce surface degradingreactions between additives in the lubricant and the steel surface, thus miti-gating the initiation of surface cracks [11, 23, 24]. Surface distress has undertest conditions been reduced in black-oxide coated samples . And thetendency for micropitting is reduced by the presence of black oxide duringrolling-sliding wear tests, when compared to untreated steel . In sum-
4The diffusion coefficient is a familiar mass transport parameter defined using Fick’slaw and with units of m2 s−1. Permeability is related to flow through a film and hasunits of molesm−1 s−1, because it represents the product of a flux (J , molesm−2 s−1) anda thickness (z, m). However, some authors define the permeability as a function of thedriving pressure p of hydrogen gas, i.e., Jz/
√p, with units molesm−1 s−1 Pa−1/2 .
5Fig. 3 in  has no scales and details are not available for scrutiny.
mary, the oxide coating may have multiple advantages, including a reductionin the infusion of nascent hydrogen into the steel and in retarding the initi-ation of surface cracks caused by reactions with lubricants.
3. Cadmium, Nickel and Alloy Plating
Cadmium is often used as a sacrificial coating on steel, especially in ma-rine environments, but its application is declining due to toxicity issues.Cadmium and tin both have a much smaller hydrogen diffusion coefficientthan ferrite, Fig. 1. It happens also to be a barrier to hydrogen permeation;Fig. 2 illustrates how the hydrogen effusion rate from previously chargedsamples of steel is dramatically reduced when coated with cadmium.
Figure 1: Diffusion coefficientsfor hydrogen in ferrite andaustenite. The dashed regionrepresents diffusion in ferritecontaining strong traps. The‘point’ is the diffusivity of hy-drogen in nickel at ambienttemperature. Data from [26–28].
Strong steels are often electroplated with cadmium or zinc as protectionagainst corrosion but the plating process itself introduces hydrogen into thesteel. It is then necessary to subject the component to a “de-embrittling”heat treatment, typically 190-230 ◦C for 8-24 h [30, 31] in order to allowdiffusible hydrogen to escape, assuming that this additional heat-treatmentdoes not compromise the other mechanical properties of the alloy. However,alloying zinc with nickel greatly reduces this penetration of hydrogen intothe steel  because nickel deposits first and forms a diffusion barrier .Nickel is a diffusion barrier to hydrogen when plated on steel; the diffusivity
Figure 2: (a) Effect of a thin layer of cadmium on the permeation of hydrogen . (b) Thehydrogen evolution rate from charged specimens of steel, in one case following cadmiumplating .
of hydrogen in nickel at room temperature is about 5 × 10−11m2 s−1 .Fig. 1 shows that at ambient temperature, the diffusivity in nickel is ordersof magnitude smaller than in ferrite, but comparable to that in ferrite con-taining strong hydrogen-traps. Nickel can therefore be applied in order toprevent the infusion of hydrogen into the steel; the plating obviously shouldbe implemented in a manner that does not to introduce hydrogen into thesteel.
Some illustrative data are presented in Table 1; in contrast to 4340 steel,the work on the 300M alloy shows only a modest improvement due to theZn-Ni coating relative to a cadmium coating. Figueroa and Robinson attribute this to the presence of defects in the Zn-Ni coating that leave someof the steel exposed, but why this is specific to 300M steel is not clear. It isspeculated that the high silicon content of 300M relative to 4340 may resultin relatively poor surface quality for coating purposes [34–37].
It is noteworthy that the passage of hydrogen through a coating dependsnot only on its diffusivity, but also the ability of adsorbed hydrogen to re-combine into molecular form and escape as bubbles before it is able to enterthe coating. Hydrogen ingress can be reduced by the presence of cadmiumin the coating because it increases this recombination rate .
Table 1: Embrittlement index, defined as 1 − (tp/tc), as a function of the type of elec-troplating. The times tp and tc are for failure of the electroplated and unplated samples.The steel compositions are given in Table 4.
Alloy Coating Embrittlement index Reference
AISI 4340, quenched & tempered Cadmium 0.78 AISI 4340, quenched & tempered Zn 0.78 AISI 4340, quenched & tempered Zn-10Ni wt% 0.037 300M, quenched & tempered Cadmium 0.54 300M, quenched & tempered Zn-14Ni wt% 0.46 
4. Other Coatings
Hard coatings such as alumina, TiC, TiN, TiO2, BN, H3PO4 glass, Cr2O3
and WC, all are in principle formidable barriers to the permeation of hydro-gen, although the actual performance depends on the structural integrity anddefect structure of the coating . And the practical utility of the coatingdepends on the service conditions. If the coated regions are subjected tolocalised stresses then the coating may wear out or detach. Typical diffusioncoefficients are illustrated in Fig. 3.
Figure 3: Hydrogen diffusiondata for TiC , TiO2 par-allel to the c-axis , Al2O3
 and Si3N4 , comparedagainst corresponding diffusivi-ties in steels from Fig. 1. γ andα refer to austenite and ferriterespectively.
In experiments on high-vacuum stainless steel systems, 1µm films of TiNhave been shown reduce the hydrogen outgassing rate from the steel by somefive orders of magnitude . Films of Cr2O3 just 3 nm thick have been
shown to present barriers to the diffusion of hydrogen ; an iron-rich oxideof the Fe2O3 type on stainless steel that is deliberately oxidised can be evenmore effective as a barrier to passage of hydrogen than the pure chromiafilm . TiC of near stoichiometric composition has a hydrogen diffusivitymany orders of magnitude smaller than that in austenite ; ZrCx, wherex ≈ 0.64− 0.81, has DH of a similar magnitude to that in TiC .
Si3N4 films of nanometre thickness have a much lower diffusivity for hy-drogen relative to steel . Ion nitriding to produce homogeneous mixturesof ε-Fe3N and γ′-Fe4N with an underlying zone rich in nitrogen also inhibitsthe penetration of hydrogen into the steel as long as the compound layer doesnot have defects that leave the steel exposed .
Alumina is particularly interesting as a hydrogen or deuterium barrierbecause it can be deposited using a variety of well-established techniques. A1µm thick layer of crystalline α-alumina deposited using a plasma technique,on a reduced-activation tempered-martensitic steel has been shown to reducethe permeation flux by a factor of 103, Fig. 4 . The coating remained ad-herent during thermal cycling to temperatures as high as 800◦C. Aluminisinginvolves the creation of a surface layer that is rich in aluminium, either insolution or present as an intermetallic compound with iron; the pack processin which the steel is heated while embedded in aluminium-rich powder canbe implemented on large components. The enriched region can be oxidisedat the surface to produce an alumina layer < 2µm thick, and since the alu-minised region is some millimetres in thickness, the alumina can in principlebe regenerated if necessary. It has been demonstrated that the presence ofalumina reduces the permeation rate of hydrogen into the underlying steelby 3-4 orders of magnitude relative to the bare steel .
Phosphorus ion implantation to produce a strengthened amorphous sur-face layer provides a diffusion barrier , possibly implying that it is difficultfor hydrogen to penetrate a disordered structure. There is evidence that thediffusion of hydrogen through an amorphous iron-base alloy is orders of mag-nitude slower than in ferritic steel , although it should be emphasisedthat the comparison is not rigorous because of the solutes added to makeiron amorphous.
Figure 4: Deuterium ‘perme-abilities’ through samples ofEurofer steel in its uncoated(bare) and coated (alumina)forms. Data from .
5. Hydrogen Trapping
Given that it is diffusible hydrogen that is damaging to steel , anymethod that renders it immobile should mitigate its effects. Darken andSmith  observed experimentally that the rate of evolution of hydrogenfrom a charged specimen is slower than the rate of absorption during charg-ing. Furthermore, a cold-rolled steel sample had a much higher saturationhydrogen content than one that is hot-rolled. It was concluded, therefore,that hydrogen can be localised at dislocations or at other “disturbances of,or departures, from the ideal lattice”. Such a non-ideal lattice would be ex-pected to impede the diffusion of hydrogen, as illustrated by the range ofvalues plotted in Fig. 1. The general and physically justifiable consensusis that strong traps reduce the susceptibility of the steel to hydrogen em-brittlement. The presence of traps does increase the saturation hydrogencontent of the steel but this trapped hydrogen is innocuous. A recent paperon X80 pipeline steel commented that the large density of traps on the steelincreases its susceptibility to hydrogen-induced cracking , but we do notbelieve this is well-founded because the comment is based on the fact thatthe steel with traps absorbs more hydrogen.
Since a trap provides a favourable environment for the hydrogen atomto reside in, there is a reduction in energy ∆E following its transfer from
a normal to a defect site  so that ∆E is negative. Trapping energieshave been widely investigated for all kinds of defects, using experimentaltechniques such as thermal desorption spectroscopy or mathematical models[54–60, e.g.]. The intention here is not to review or assess trapping energies,but rather to focus on how such traps might be exploited in order to miti-gate hydrogen embrittlement. It is generally accepted that modification ofthe transport rate of hydrogen is a promising route to improving hydrogencompatibility .
It is worth noting here that using the concept of exploiting hydrogentraps to make steels more resistant to hydrogen embrittlement was in partstimulated by the observation of delayed fracture in strong steels that aresubjected to hydrogen ingress. Delayed fracture occurs when a steel sub-jected to a stress that is small relative to its fracture strength measured onmanufacture, undergoes spontaneous brittle failure after a period of time inservice . This failure under static load is attributed to the presence ofhydrogen. Fig. 5 shows how the fracture strength decreases with time in sam-ples that have been charged electrolytically with hydrogen. The data showthat for any component loaded initially at a stress greater than 600MPa,fracture would occur after a short period in service .
Figure 5: Fracture stressfor samples of strong steelthat have been electrolyti-cally charged with hydrogen.The steel has the chemicalcomposition Fe-0.39C-0.76Mn-0.28Si-1.8Ni-0.75Cr-0.24Mowt%, with a 0.2% proofstrength of 1516MPa. Datafrom .
5.1. Reversible and Irreversible Traps
In the present context, irreversible implies that trapped hydrogen is notable to re-enter the lattice and contribute to diffusible hydrogen during theservice conditions and during the intended service life of the steel. This def-inition is somewhat different from specifying a particular trap energy thatdistinguishes reversible from irreversible traps [62, e.g.] because such a pro-cedure fails to account for time and environment. In a thermal desorption ex-periment, hydrogen evolved at a low temperature is weakly trapped whereasthe ‘irreversibly’ trapped hydrogen is only released at higher temperatures.However, the actual temperature at which significant quantities of hydrogenare detrapped, depends also on the heating rate, emphasising the role oftime. The equilibrium between trapped hydrogen and that dissolved in thematrix means that when the latter escapes, that which is trapped will re-lease hydrogen to re-establish equilibrium, a phenomenon confirmed directlyusing autoradiography . As pointed out by Maroef et al. , a trapwith a binding energy of 100 kJmol−1 is considered irreversible at ambienttemperature but becomes reversible at a sufficiently high temperature.
The distinction between reversible and irreversible traps becomes particu-larly important when modelling the effect of hydrogen on mechanical proper-ties. The quantitative effect is expressed as an empirical hydrogen influencefactor [64–66] that then is incorporated into expressions for the fatigue crackgrowth rate. The influence factor is defined differently for diffusible and non-diffusible hydrogen, with a working assumption that the hydrogen releasedunder ‘ambient conditions’ is classified as diffusible .
Typical traps for hydrogen and the associated binding energies (Eb) arelisted in Table 2, with the definition of Eb illustrated in Fig. 6. It is suggestedthat permeation experiments directly yield Eb whereas thermal desorptiongives the combination Eb+Q, where Q is the activation energy for hydrogendiffusion . This may not strictly correct if the appropriate theory isused to interpret thermal desorption experiments so that Eb can be obtaineddirectly . Kissinger’s reaction rate theory  is widely applied to derivea detrapping activation energy (Eb +Q), but it is not fit for purpose since itdeals with homogeneous reactions, whereas the experiments involve diffusiontowards the sample surface. There is nothing in the theory regarding sampleshape and size. McNabb and Foster’s model , on the other hand, explicitlyhandles Q and Eb and therefore is able to deal with the capture and release
of hydrogen from traps, and its diffusion through the lattice. There will,in any event, be considerable uncertainties in the measurement of Eb for alltechniques since much of the theory is applied as if there is a single typeof trap site, whereas in practice a real material will contain a variety oftraps and a spectrum of binding energies. This kind of a problem is besthandled numerical or computational methods as in [68, 71]. In spite of theseuncertainties in the absolute values of Eb, it is likely that the rankings oftrap potencies are reasonable; for example, a dislocation core is expected tobe a deeper trap for hydrogen than its elastic strain field (Table 2).
Table 2 also lists the trapping ability of individual solutes. The bind-ing energies quoted are likely to be reliable as far as the separation of theactivation energy of diffusion and Eb is concerned, because they come fromcalculations or magnetic relaxation methods. Furthermore, those deduced us-ing techniques such as thermal desorption spectroscopy may not be rigorousbecause the solutes also cause microstructural changes and hence trappingtendencies; this is reflected, for example, in the study of the role of tungstenon hydrogen trapping .
Voids into which hydrogen locates and combines to form the molecularvariety would in general fall into the irreversible category because the molec-ular hydrogen would need to dissociate before it can re-enter the iron lattice.On the other hand, although carbon atoms dissolved in the steel have an as-sociation with hydrogen , they represent weak traps ; if the diffusiblehydrogen in the lattice reaches a concentration below that expected in equi-librium with such a trap, then the hydrogen would be expected to re-entersolution.
Even weak traps reduce the ability of hydrogen to diffuse through thesteel. Thus, water-quenched, martensitic 2.25Cr1Mo steel has an apparenthydrogen diffusivity at ambient temperature, as measured by permeation, tobe DH = 0.21-0.31 × 10−10m2 s−1. After tempering at 640◦C to generate avariety of carbides, the diffusivity increases to DH = 0.29-0.47×10−10m2 s−1,but the quantity of irreversibly trapped hydrogen increases by about an orderof magnitude relative to the untempered state .
Table 2: Published data on trapping (binding) energies Eb for hydrogen or deuteriumatoms in ferritic steels. Notice that nickel in ferritic iron (α) repels hydrogen. Austeniteis labelled ‘γ’. The binding energies have been rounded off to integers. It should benoted that the strain field of a dislocation is reduced by the segregation to it of carbonor nitrogen, so the tendency for trapping hydrogen also diminishes . († quoted fromthe secondary source ; it has not been possible to obtain the original paper ). Thehydrogen located at microscopic voids is believed to be in molecular form so it is not clearwhy the trapping energy is so small. ‘TDA’ stands for thermal desorption analysis. ‘M’represents metal atoms.
Trap site Phase −Eb/kJmol−1 Method Reference
Single iron-vacancy α 49–78 Diffusion analysis [78–80]Single iron-vacancy α 24-29 First principles calculations Cr, Mo or V atom α 26–27 Elastic/electronic calculations Mn atom α 11 Elastic/electronic calculations Ni atom α −12 Elastic/electronic calculations C atom α 3 Magnetic relaxation N atom α 13 Magnetic relaxation Al atom γ 6 First principles calculation Ti atom α 26 Permeability 
General grain boundaries α 32 Mechanical analysis γ/α interface γ + α 52 Permeability Dislocation strain field α 23-27 Diffusion analysis, TDA [86–88]Dislocation core/jogs α 60 Diffusion analysis Microvoids α 48 Thermal desorption analysis 
ε-carbide α 65 †Cementite/α interfaces α 11-18 Permeability, TDA [88, 91]TiC α 46-116 Permeability [54, 92, 93]Fe1.2Ti0.8S2 α 58 Thermal desorption spectroscopy V4C3 α 33-35 Thermal desorption analysis Coherent M2C (Mo-rich needles) α 11-12 Thermal desorption analysis MnS α 72 †MnS/α interfaces α 72 Thermal desorption analysis [87, 90]Iron oxide/α interfaces α 51-70 Thermal desorption analysis Y2O3/α interfaces α 70 Thermal desorption analysis [58, 98]Al2O3/α interfaces α 79 Thermal desorption analysis 
Figure 6: Illustration of thebinding energy, and activationenergy of diffusion in the per-fect lattice.
6. Atomic Traps
We have seen from the data presented in Table 2 that individual atomscan attract hydrogen atoms but the mechanism of trapping can vary, andeach solute atom is not in general likely to attract more than a couple ofhydrogen atoms.
The chemical affinity of titanium for hydrogen is known to be potent.Hydride precipitation is possible in titanium based alloys and because thereaction is reversible, hydrides have been proposed for large scale hydrogenstorage systems. Pressouyre and Bernstein  demonstrated that titaniumatoms in Fe-Ti ferritic alloys can act as low-occupation traps with −EB ≈26 kJmol−1.
High-manganese twinning-induced plasticity steels (TWIP, typically Fe-18Mn-1.5Al- 0.6C wt%) exhibit combinations of elongation and strength thatmight be attractive [100–102] but can be susceptible to delayed, hydrogen-induced failure [103–108]. However, it is known that adding less than 2wt%of aluminium ameliorates the situation [60, 109]. Possible mechanisms of therole of aluminium include:
• suppression of strain ageing due to carbon, with the resulting reductionin the flow stress making hydrogen embrittlement less likely .
• Aluminium might reduce the absorption of hydrogen [111, 112] butthis is inconsistent with experimental data [113, 114] that indicate theopposite effect.
• Phase transformation into ε-martensite, or mechanical twinning, maymitigate hydrogen effects .
• Hydrogen reduces the shear modulus of the austenite whereas alu-minium has the opposite effect in the presence of hydrogen. This mightin some way relate to hydrogen embrittlement .
There is a further explanation that is generic to ferritic and austenitic steels,that aluminium influences binding energies and the local density around thealuminium atoms. Thus, in the context of low-alloy steels, first principlescalculations show that aluminium-alloyed ferrite should be more resistantto hydrogen than that which has silicon added . In austenite, the dis-tance between a substituted aluminium atom and the adjacent iron atomis greater than between a corresponding pair of iron atoms (Fig. 7a). Thisadditional space makes an atom of aluminium a weak trap with a bindingenergy of 6 kJmol−1, which is the reason why the aluminium-alloyed TWIPsteel absorbs more hydrogen in charging experiments (Fig. 7b).
7. ε-carbide and Cementite
Fukui et al.  studied the delayed fracture behaviour of six differentsteels following immersion in a 0.1N HCl solution for 30 h. They characterisedthe response with the ratio of the fracture strength measured following im-mersion, to the strength determined in the unexposed samples. The steelswere quenched and then tempered at a variety of temperatures, in all casesfor 1 h. Two of the steels studied had similar carbon concentrations in therange 0.2-0.21wt%, but quite different silicon contents at 0.27 and 0.75wt%.It was noted that both steels exhibited favourable peaks in the embrittlementratio,6 with the peak at 250◦C (Fig. 8) in the low-silicon alloy and at 300◦Cfor the higher silicon steel. They suggested that this is because ε-carbidesform during low-temperature tempering, but when the silicon concentration
6This ratio is sometimes known as the ‘delayed fracture ratio’.
Figure 7: (a) Atomic structure of Fe31Al with the distance between nearest atom. Thered arrows indicate the same distance between Al and Fe atom. The fractions indicate theheight of the atom in the direction normal to the diagram; unlabelled atoms are at heights0,1. (b) The reported and predicted hydrogen thermal desorption rate of austenite andAl containing austenite  , together with the calculated curves based on the trappingenergy calculated using first principles methods.
is greater, the precipitation is retarded to 300 ◦C. Silicon is known to retardthe conversion of transition carbides such as ε-carbide into cementite [117–123], because of its incredibly low solubility in cementite that is in equilibriumwith austenite [124–126] and ferrite .
Figure 8: Ratio of the frac-ture strength at 30 h to thestatic strength, as a functionof the tempering temperaturewith the tempering time fixedat 1 h. Adapted from .
If ε-carbide is a more effective hydrogen-trap than cementite, then thiswould explain the shift of the peak in the delayed fracture embrittlementratio to higher temperatures in the silicon-rich steel, Fig. 8. It is reasonableto argue that ε-carbide would be more effective than cementite particles ofthe same size, in trapping hydrogen. This is because it has a lower interfacialenergy with the ferrite and its coherency or semi-coherency with the matrixresults in strain fields that attract and pin hydrogen . ε-carbide is notthermodynamically stable relative to Fe3C, and yet forms first because ofthis coherency which reduces the activation energy for nucleation. Not sur-prisingly, cementite formed by quenching and tempering a 0.2wt% C steelhas been reported to have a negligible effect on the trapping of hydrogen and a similar conclusion was reached in a higher carbon steel .Ferrite-cementite interfaces are weak traps (Table 2, ). Indeed, cementitein the absence of a significant trapping capacity can be positively harmful ininitiating hydrogen-induced cracking .
ε-carbide as a phase can absorb hydrogen and even form a compoundFe2HC, in addition to acting as a trap via its coherency strain fields . The
evidence for this comes from experiments where the hydrogen content of thecarbide has been chemically analysed . Recent atom-probe tomography,Fig. 9, has revealed the segregation of hydrogen to ε-carbide, and the dataseem to suggest that the hydrogen is in fact inside the carbide particles .
The amount of hydrogen associated with incoherent TiC particles seemsto correlate with the volume of the carbide, indicating that it too is capableof absorbing hydrogen within its structure . In this case, the hydrogenis apparently trapped at carbon-vacancies within the lattice. Small, semi-coherent TiC particles have fewer such vacancies and hence their trappingmechanism is primarily through interface structure and strain fields.
Figure 9: Atom probe datataken across an ε-carbide par-ticle in a hydrogen-containingsteel. The inset shows thecorrelation between the hydro-gen and carbon concentration.Adapted from .
The general conclusion that cementite-ferrite interfaces represent inef-fective traps for hydrogen (Table 2, [88, 91]) with EB of the order of 11-18 kJmol−1 is not consistent with ab initio calculations that suggest EB ≈47 kJmol−1 . However, the calculations may not be representative be-cause the interface studied had to be made coherent due to the nature of themethod used, by artificially implementing a huge adjustment to particularlattice parameters.
8. Substitutionally-Alloyed Carbides and Nitrides
The carbide particles that precipitate at temperatures where substitu-tional solutes such as molybdenum, vanadium, niobium and titanium becomemobile over length scales of a few nanometres are particularly interestingfrom the point of view of hydrogen trapping. With appropriate temperingat temperatures in the range 500-600 ◦C, the distance over which the atomswill move is in the range 1-1000 nm [135, p. 74] for typical tempering times.This means that the carbide dispersion can be carefully controlled while atthe same time selecting tempering conditions that are suitable for the otherproperties required of the steel .
Vanadium based carbides have long been known to be effective in miti-gating hydrogen-induced delayed fracture in strong bolting steels. The bind-ing energy determine using thermal desorption analysis is found to be 33-35 kJmol−1. It has been argued  that the key trap in V4C3 is at carbonvacancies in the lattice, but the binding energy calculated for this is not con-sistent with that measured; furthermore, it has been demonstrated that thestate of coherency with the ferrite influences the hydrogen trapping capacity, emphasising the role of the strain fields around the carbides. Atom-probe data, although uncertain,7 appear to show deuterium segregation tothe interface  rather than within the carbide itself.
ε-Ti(C,N) carbonitrides with a tetragonal unit cell and the orientationrelationship:
[1 1 1]α ∥ [3 4 2]ε−Ti(C,N) (1 1 0)α ∥ (2 2 1)ε−Ti(C,N)
have a high degree of coherence with the ferritic (α) matrix.8 Permeation ex-periments have shown that in enamelling steel (Table 3) they form hydrogentraps whereas Ti(C,N) with a face-centred cubic structure or TiS particles areincoherent and do not contribute to the trapping phenomenon . This,however, is not a generic conclusion because there is ample evidence that the
7There is an interesting discussion about the uncertainties of measuring hydrogen inthe atom probe , together with evidence for hydrogen trapping at a precipitate in analuminium alloys.
8The plane indices (2 2 1) are a correction of the original (2 2 1) so that the angle betweenthe plane normal and direction [3 4 2] becomes 90◦, as is it for the corresponding indicesin ferrite.
Table 3: Compositions (wt%) of some of the steels containing substitutional solutes toform alloy carbides that trap diffusible hydrogen and hence increase the resistance toembrittlement.
Alloy C Si Mn Ni Mo Cr V Nb Others Reference
Bolt steel, quenched, tempered550-650◦C for 90min.
0.5 0.3 0.7 1.0 0.3 0.03 
Bolt steel, without vanadium,quenched and tempered at 500-550◦C for 90 min.
0.39 0.82 0.16 1.11 - 0.03 
Bolt steel with molybdenum car-bides (NIMS17), quenched, tem-pered at 570◦C, 90min
0.59 1.98 0.20 0.94 0.99 [141–143]
Enamelling steel 0.048 0.05 0.47 0.3Ti, 0.0046 N 
Figure 10: Comparison of thesusceptibility to delayed frac-ture, of two bolting steels whosedetailed chemical compositionsare given in Table 3. The steelwith vanadium contains vana-dium carbides that serve to trapotherwise diffusible hydrogen,thus dramatically reducing itsapparent diffusivity D. There-fore, the embrittlement ratio ismuch larger with the vanadium-containing steel, a higher ratioimplying that the static frac-ture strength is less affected byhydrogen. Data from .
most powerful traps are associated with the incoherent TiC particles, with−EB ranging from 46-116 kJmol−1 depending on the state of coherency [e.g.,
92]. But it is worth emphasising that the crystal structures of the titaniumcarbides are often not reported.
Figure 11: The horizontal linesrepresent the sequence of ionsentering the time of flight massspectrometer of an atom probe,with the probe hole placed atthe TiC/ferrite interface. Onlythe deuterium and hydrogenions are plotted, the Fe, C, Tiomitted for clarity. No deu-terium atoms were detected inthe sequence far from the inter-face. The far field is not illus-trated here but is available in from which this figure isadapted.
The first direct determination of a hydrogen isotope, deuterium, at acoherent TiC/ferrite interface using the atom probe was by Spitzangel etal. , Fig. 11. It is interesting that the titanium carbide contains somehydrogen, though not deuterium. In a more recent experiment using a tomo-graphic atom probe, deuterium was used in order to distinguish from hydro-gen present in the instrument itself ; this work confirmed the segregationof deuterium in the proximity of the small titanium carbides. Spitzangel etal. suggested that it would be useful to examine larger, incoherent particles,to see whether the particles themselves contained hydrogen.
Atom probe tomography has been reported for deuterium segregation inthe proximity of V4C3 precipitates . Similar results have been reportedfor ε-carbide because there is a strong correlation between the carbon andhydrogen concentrations . Fig. 12 shows two examples of experimentsthat demonstrate that carefully designed vanadium-molybdenum carbide canbe very effective in trapping hydrogen. In the case of the bearing steel SUJ2[147, 148], the sample was tested immediately after charging and it was estab-lished using a control experiment where the sample was heated at 3Kmin−1,that the peak below about 150 ◦C is due to the evolution of diffusible hy-drogen. Data confirming the attribution of this peak to diffusible hydrogenare available also for lower carbon quenched and tempered steels  and
for pure iron and eutectoid steels . The actual temperature range overwhich diffusible hydrogen is released will depend on the heating rate and sam-ple size used in thermal desorption analysis.9 The subsequent smaller peakat temperatures in excess of 350 ◦C corresponds to the release of trappedhydrogen, although the nature of the traps was not stated.
The second steel is not a bearing alloy, and is tested after allowing thediffusible hydrogen to escape from the 8mm diameter samples by holdingat 20 ◦C for 100 h . It is heat treated to precipitate fine particles of(V,Mo)4C3 which through their coherency strain fields are able to trap hy-drogen. The peak corresponding to this particular alloy therefore representsonly the trapped hydrogen.
Figure 12: Hydrogen evolu-tion rates. Both alloys werecathodically charged with hy-drogen at 0.2mA cm−2. (a)A standard bearing steel [148,Table 1], charged for 20 hand then immediately testedfor hydrogen evolution .(b) An alloy containing co-herent (V,Mo)4C3 hydrogen–trapping precipitates, chargedfor 48 h, and tested after allow-ing diffusible hydrogen to es-cape .
8.1. Efficacy of Traps
While traps undoubtedly reduce the mobility of hydrogen atoms in ferriteor austenite, in circumstances where the amount of hydrogen that enters thesteel is large, they actually increase the uptake of hydrogen. Given that thetrapped hydrogen will be in local equilibrium with the lattice, if EB is small,then it would be easy for the trap to act as a source of diffusible hydrogen
9A useful practical definition of diffusible hydrogen is that which escapes when the steelis left at room temperature for several days .
if the concentration in the matrix becomes depleted below the equilibriumvalue. The traps in these cases would not mitigate the embrittlement of thesteel. Akiyama  pointed out that a particular bolting steel (Table 3)containing molybdenum carbides did not show exceptional resistance to hy-drogen embrittlement in cyclic corrosion tests because of the high hydrogenuptake of the steel . The molybdenum carbides are relatively weak traps(Table 2) and hence the supply of diffusible hydrogen would be maintainedby equilibrium with the matrix. In order for traps to be effective, they musthave a large enough binding energy so that the equilibrium concentrationof diffusible hydrogen in the matrix is much smaller than required to causeembrittlement.
It has been suggested that there is a critical diffusible-hydrogen concen-tration HC below which delayed fracture does not occur for a steel with themicrostructure defined. This is determined experimentally. If the amount ofhydrogen that enters the steel from the environment, HE, is less than HC,then delayed fracture is said not to occur in service [29, 152, 153]. So theproblem reduces to one in which the steel and its heat treatment are designedto maximise HC, possibly by using hydrogen trapping carbides. In the workdescribed in the preceding paragraph , laboratory experiments were per-formed in which samples were charged with hydrogen, rather than exposedto an environment. Therefore, the traps would have been saturated, andsubsequently served as sources for hydrogen. What really is needed in orderto assess the efficacy of traps is a reliable measure of HE and this presumablycannot be achieved without exposure in an actual service environment. Taruiet al.  claim that there is little correlation between accelerated tests (us-ing hydrogen charging) and performance in actual environments. Fig. 13 isa particularly useful extract from more comprehensive data , becausethe bolt did not contain diffusible hydrogen, only trapped hydrogen and ina quantity that turned out to be very small, at about 0.2 p.p.m. This isimportant to note because numbers like these define the trap capacity thatmust be built into bolts in order to avoid delayed fracture.
Although some inclusions such as MnS are associated with large trappingenergies (Table 2), the inclusions themselves can harm the overall propertiesdepending on their size and distribution. It has, for example, been concludedthat the experimentally observed accumulation of hydrogen around MnS in-clusions is responsible for failure in fatigue testing . This applies also tofatigue initiated at oxide inclusions [156, 157]. Therefore, inclusions that are
Figure 13: Thermal desorptiondata for hydrogen in a typi-cal high-strength bolt that hasbeen used on a bridge for fiveyears.
weakly bonded to the steel and at the same time initiate fracture because oftheir size, are not suitable as deliberate hydrogen traps. As emphasised inthe introduction, it is the benign traps such as the semi-coherent carbidesthat should be exploited in this context.
9. Retained Austenite and Hydrogen Mobility
In a study of two quenched and tempered martensitic steels, Figueroaand Robinson  concluded that martensite which is surrounded by retainedaustenite is more resistant to hydrogen embrittlement because the austenite isa sink for hydrogen. AerMet 100 (Table 4) often contains austenite that formsby reversion during the seondary-hardening heat treatment; this correlateswith the absence of significant embrittlement following electroplating. Incontrast, the same treatment causes a large loss of toughness at comparablestrength, in 300M steel which does not contain austenite in its microstructure.
Retained austenite is able to act as a trap for three reasons, first that thesolubility of hydrogen is greater in that phase, secondly the low rate at whichhydrogen can diffuse in austenite, and thirdly, the γ/α interface is a strongtrap  so that once the hydrogen enters the austenite, it is more difficultfor it to leave. The ability of retained or reverted austenite to absorb excesshydrogen has been repeatedly demonstrated [33, 158–164, e.g.]. It should benoted that if the austenite during service transforms into brittle martensite,the latter would inherit the hydrogen concentration of the austenite, whichis likely to be detrimental to overall properties .
Retained austenite also reduces the overall diffusivity and permeabilityof hydrogen through the steel [159, 165]. Following , if ferrite can becompletely surrounded by austenite, then the mobility of hydrogen throughthe structure should be greatly reduced. Nanostructured bainite forms theideal test material for this concept given that the amount of retained austen-ite which is present as thin films is above the percolation threshold. Fig. 14shows first that the diffusivity of hydrogen increases sharply as the retainedaustenite content falls below the threshold value of V γ
V ≈ 0.1 in nanostruc-tured bainite . Secondly, the duplex steel contains the largest amount ofaustenite but its morphology is such that there is a continuous path throughthe ferrite, thus leading to a greater diffusivity than the nanostructured bai-nite with austenite fraction greater than the percolation threshold.
When the austenite fraction or its morphology is such that it does notpercolate sufficiently to surround the ferrite, it nevertheless requires the hy-drogen to follow a tortuous path through the ferrite. In duplex steels thishas been shown to reduce the effective diffusivity by a factor of two 
Figure 14: The diffusion coefficient forhydrogen through nanostructured bai-nite (circles) and a different duplex steelwhere the austenite does not percolate(square). The amount of austenite in thenanostructured bainite was controlled bytempering heat treatments. α and γ rep-resent ferrite and austenite respectively.After .
A comparison of the reduction in tensile ductility in samples charged withhydrogen indicates that the nanostructured bainite has a greater resistanceto embrittlement when compared with a quenched and tempered martensiticmicrostructure produced in the same steel . The experiments were de-signed to test both the martensitic and bainitic structures at approximatelythe same strength level. The better resistance of the bainite was attributed
to the presence of retained austenite and a large density of interfaces thatmight trap hydrogen.
Finally, it is noteworthy that hydrogen per se does not influence thestability of the austenite .
Table 4: Chemical compositions of steels in wt%.
Alloy C Si Mn Ni Mo Cr V Co Others Ref.
4340 0.41 0.23 0.79 1.67 0.22 0.88 300M 0.4 1.6 0.7 1.8 0.25 0.8 AerMet 100 0.23 11.5 3.1 13.5 
10. Lath boundaries
In a comparison of a variety of linepipe steel (0.05wt% C) microstruc-tures, permeation experiments established that bainite and acicular ferritemicrostructures are far more effective in trapping hydrogen than ferrite-pearlite mixtures . The measured apparent diffusivities were reducedby a factor of two by the trapping of hydrogen at the finely dispersed ce-mentite/lath interfaces. This led to a significant increase in the resistance tohydrogen induced cracking. In that study , cracks were found to nucle-ate at martensite-austenite boundaries (the so-called MA constituent). In ahigher carbon steel containing three times as much carbon (0.15wt% C), themicrostructure at the lath boundaries was in addition found to be effective intrapping hydrogen, but cracks also initiated at those boundaries, presumablybecause of the coarser cementite particles , and as a consequence, thetendency to crack normal to the lath boundaries.
That hydrogen embrittles iron, both austenitic and ferritic, is in no doubtand it does so at incredibly low average concentrations. It has been knownsince 1875 that it is diffusible hydrogen that is harmful. The conventionalwisdom is that diffusion is necessary so that the hydrogen can concentrateat stress concentrations such as the tips of sharp cracks and therefore hasgreater consequences than indicated by a low average concentration.
Fig. 15 illustrates the key mechanisms that exist to ameliorate the effectsof hydrogen in steel. A plethora of coatings exist that have been demon-strated to reduce either the outgassing of hydrogen in vacuum systems, or asdiffusion barriers to the ingress of hydrogen. However, the choice of coatingsavailable decreases when the coating has to perform multiple functions, forexample to resist abrasion and impact. Coatings will contain defects thatlocally expose the steel; some sort of a sacrificial mechanism is then calledfor as in the case of the Zn-Ni coatings. The thickness and integrity of thecoating will vary with the manufacturing process and has to be compatiblewith the service conditions of the protected component. The quality of thecoating can depend on the chemical composition and structure of the sub-strate. Ion implantation can be used to favourably alter the surface of thesteel.
Some phases within steels can actually soak-up hydrogen, for example theε-carbide; however, retained austenite which is common in steels may be themost promiscuous hydrogen sink. In TRIP steels the austenite usually con-tains a large carbon concentration and is designed to transform into marten-site under the influence of stress or plastic strain. The martensite wouldthen inherit the hydrogen concentration present originally in the austen-ite and this may compromise the overall properties. Reverted austenite inmarageing steels or in secondary-hardened steels containing a stoichiometricconcentration of carbon are not expected to suffer from this difficulty becauseof the zero or low carbon concentration of the alloys.
Retained austenite can have a different function, that of acting as a diffu-sion barrier to hydrogen in predominantly ferritic steels. However, its volumefraction must be above a percolation threshold so that the ferrite is micro-scopically isolated. Even when the fraction is below the percolation thresh-old, the austenite can increase the tortuousity of the path that the hydrogenmust follow through the structure, and hence reduce its ingress.
There are many varieties of strong hydrogen traps in steels, but by far themost advanced application of the concept of capturing diffuisible hydrogenwithin the steel has been in the invention of strong bolting steels that are notsusceptible to delayed fracture. The bolts have been tested for many yearsin service and demonstrated to outperform those that do not contain thehydrogen traps. Furthermore, even after years of service, the bolts in theiroperating environment were found to contain less than 1 p.p.m. of hydrogen.
Figure 15: Mechanisms available for the modification of steel to better resist hydrogen.
The actual trapping capacity from the vanadium carbides is in fact muchgreater that that.
 W. H. Johnson: Proceedings of the Royal Society of London, 23 (1875) 168–179. E. Serra, A. Perujo, G. Benamati: Journal of Nuclear Materials, 245 (1997) 108–114. M. Wang, E. Akiyama, K. Tsuzaki: Corrosion Science, 49 (2007) 4081–4097. G. T. Park, S. U. Koh, H. G. Jung, K. Y. Kim: Corrosion Science, 50 (2008)
1865–1871. Y. D. Han, H. Y. Jing, L. Y. Xu: Materials Chemistry and Physics, 132 (2012)
216–222. L. P. Pfeil: Proceedings of the Royal Society of London, 112 (1926) 182–195. L. S. Darken, R. P. Smith: Corrosion, 5 (1949) 1–16. G. M. Pressouyre: Metallurgical & Materials Transactions A, 14 (1983) 2189–2193. R. M. Hurd, N. Hackerman: Journal of the Electrochemical Society, 104 (1957)
482–485. L. H. Wagner: Corrosion resistance of black oxide coatings on mild and corrosion
resistant steel: Tech. Rep. 64-3580: Rock Island Arsenal Laboratory: Illinois, USA(1964).
 K. Stadler, B. Han, V. Brizmer, R. Pasaribu: Technology Evolution, No. 2 (2015)25–30.
 K. Nomura: Mossbauer spectroscopy in materials science: Springer, Netherlands,1999: Ch. 4: pp. 63–78.
 R. H. Wolff: Hydrogen embrittlement of steel in metal finishing processes of blackoxide and zinc phosphate: Tech. Rep. 66-2008: Rock Island Arsenal Laboratory:Illinois, USA (1966).
 R. D. Evans, C. H. Hager, R. D. Logsdon: Friction and wear performance of can-didate surface treatments for wind turbine gearbox bearings in high slip contacts:in: International Joint Tribology Conference: IJTC2009-15206, ASME, New York,USA, 2009: pp. 1–3.
 R. D. Evans, C. H. Hager Jr., Y. S. Kang, G. L. Doll: Tribology Transactions, 58(2015) 444–453.
 A. A. bin Ahmad Fauzi: Production of magnetite thin film over steel substrate usinghot alkaline nitrate blackening method: Master’s thesis: Universitat Politecnica deCatalunya: Barcelona, Spain (2014).
 R. Errichello, S. Sheng, J. Keller, A. Greco: Wind turbine tribology seminar: Tech.Rep. DOE/GO-102012-3496 February 2012: U. S. Department of Energy: Golden,Colorado, USA (2012).
 R. H. Song, S. I. Pyung, R. A. Oriani: Electrochimica Acta, 36 (1991) 825–831. B. Han, B. X. Zhou, R. Pasaribu: C-ring hydrogen induced stress corrosion cracking
test in lubricating liquid media: in: Proceedings of European Corrosion Congress:Stockholm, Sweden, 2011: pp. 615–623.
 D. Khatamian, F. D. Manchester: Journal of Nuclear Materials, 166 (1989) 300–306. G. W. Hollenberg, E. P. Simonen, G. Kalinin, A. Terlain: Fusion Engineering and
Design, 28 (1995) 190–208. E. Serra, G. Benamati: Materials Science and Technology, 14 (1998) 573–578. M. Reichelt, T. E. Weirich, J. Meyer, T. Wolf, J. Loos, P. W. Gold, M. Fajfrowski:
Journal of Material Science, 41 (2006) 4543–4553.
 H. R. Pasaribu, P. M. Lugt: Tribology Transactions, 55 (2012) 351–356. B. Mahmoudi, B. Tury, C. H. Hager, G. L. Doll: Tribology Letters, 58 (2015) 1–9. F. R. Coe: Welding steels without hydrogen cracking: Tech. rep.: The Welding
Institute: Abingdon, U. K. (1973). M. L. Hill, E. W. Johnson: Acta Metallurgica, 3 (1955) 566–671. M. Zamanzadeh, A. Allam, C. Kato, B. Ateya, H. W. Pickering: Journal of the
Electrochemical Society, 129 (1982) 284–289. S. Yamasaki, T. Takahashi: Tetsu-to-Hagane, 83 (1997) 454–459. M. P. Nascimento, R. C. Souza, W. L. Pigatin, H. J. C. Voorwald: International
Journal of Fatigue, 23 (2001) 607–618. E. M. K. Hillier, M. J. Robinson: Corrosion Science, 48 (2004) 715–727. M. J. Carr, M. J. Robinson: Trans. IMF, 73 (1995) 58–64. D. Figueroa, M. J. Robinson: Corrosion Science, 50 (1066-1079). T. Fukagawa, H. Okada, Y. Maehara: ISIJ International, 34 (1994) 906–911. H. Okada, T. Dukagawa, A. Okamoto, M. Azuma, Y. Matsuda: ISIJ International,
35 (1995) 886–891. S. Taniguchi, K. Yamamoto, D. Megumi, T. Shibata: Materials Science & Engi-
neering A, 308 (2001) 250–257. E. J. Song, D. W. Suh, H. K. D. H. Bhadeshia: Ironmaking and Steelmaking, 39
(2012) 599–604. H. Kim, B. N. Popov, K. S. Chen: Corrosion Science, 45 (2003) 1505–1521. Y. Hatano, T. Nozaki, H. Homma, M. Matsuyama: Diffusion behaviour of hydrogen
in TiC: in: Annual Report of Hydrogen Isotope Research Center: Vol. 26: ToyamaUniversity, Japan, 2006: pp. 31–43.
 J. B. Bates, J. C. Wang, R. A. Perkins: Physical Review B, 19 (1979) 4130–4139. A. B. Belonoshko, A. Rosengren, Q. Dong, G. Hultquist, C. Leygraf: Physical Review
B, 69 (2004) 024302. G. C. Yu, S. K. Yen: Applied Surface Science, 201 (2002) 204–207. K. Saito, Y. Inayoshi, Y. Ikeda, Y. Yang, S. Tsukahara: Journal of Vacuum Science
& Technology, 13 (1995) 556–561. M. Takeda, H. Kurisu, S. Yamamoto, H. Nakagama: Vacuum, 84 (2010) 352–356. Y. Ishikawa, T. Yoshimura: Journal of Vaccum Science and Technology, 13 (1995)
1847–1852. Y. Hatano, T. Nozaki, H. Homma, M. Matsuyama: Absorption and release of hy-
drogen isotopes by ZrC: in: Annual Report of Hydrogen Isotope Research Center:Vol. 27: Toyama University, Japan, 2007: pp. 27–36.
 P. Bruzzoni, S. P. Br’uhl, B. A. Gomez, L. Nosei, M. Ortiz, J. N. Feugeas: Surfaceand Interface Analysis, 110 (1998) 13–18.
 D. Levchuk, F. Koch, H. Maier, H. Bolt: Journal of Nuclear Materials, 328 (103-106).
 K. S. Forcey, D. K. Ross, C. H. Wu: Journal of Nuclear Materials, 182 (1991) 36–51. W. Ensinger, G. K. Wolf: Nuclear Instruments and Methods in Physics Research
Section B: Beam Interactions with Materials and Atoms, 39 (1989) 552–555. D. S. Dos Santos, P. V. De Miranda: Journal of Materials Science, 32 (1997) 6311–
 J. Dong, H. Vetters, F. Hoffmann, H. W. Zoch: Journal of ASTM International, 7(2010) JAI 102511.
 R. A. Oriani: Acta Metallurgica, 18 (1970) 147–157. G. M. Pressouyre, I. M. Bernstein: Metallurgical transactions A, 9 (1978) 1571–1580. J. P. Hirth: Metallurgical & Materials Transactions A, 11 (861-890). P. Nordlander, J. K. Norskov, F. Besenbacher: Journal of Physics F: Metal Physics,
16 (1986) 1161–1171. R. Griessen: Physical Review B, 38 (1988) 3690–3698. I. Maroef, D. L. Olson, M. Eberhart, G. R. Edwards: International Materials Re-
views, 47 (2002) 191–223. S. Frappart, A. Oudriss, X. Feaugas, J. Creus, J. Bouhattate, F. Thebault, L. De-
lattre, H. Marchbois: Scripta Materialia, 65 (2011) 859–862. D. W. Suh: Materials Science and Technology, 30 (2014) 1131–1134. R. P. Frohmberg, W. J. Barnett, A. R. Troiano: Delayed failure and hydrogen
embrittlement in steel: Tech. Rep. 54-320: Wright-Patterson Air Force Base: Ohio,U. S. A. (1954).
 T. Michler, M. P. Balogh: International Journal of Hydrogen Energy, 35 (2010)9746–9754.
 G. Katano, K. Ueyama, M. Mori: Journal of Materials Science, 36 (2001) 2277–2286.
 Y. D. Li, Z. G. Yang, Y. B. Liu, S. X. Li, G. Y. Li, W. J. Hui, Y. Q. Weng: MaterialsScience & Engineering A, 489 (2008) 373–379.
 Y. Li, Z. Yang, S. Li, Y. Liu, S. Chen, W. Hui, Y. Weng: Advanced EngineeringMaterials, 11 (2009) 561–567.
 Y. D. Li, W. M. Guo, N. Xu, X. F. Wu, J. B. Shi, H. Ma: Materials Science andTechnology, 30 (2013) 1463–1469.
 J. B. Shi, Y. D. Li, W. M. Guo, N. Xu, X. F. Wu, M. Zhao, H. Ma: MaterialsScience and Technology, 29 (2013) 1290–1296.
 E. J. Song, D. W. Suh, H. K. D. H. Bhadeshia: Computational Materials Science,79 (2013) 36–44.
 H. E. Kissinger: Analytical Chemistry, 29 (1957) 1702–1706. A. McNabb, P. K. Foster: Trans. AIME, 227 (1963) 618–627. M. Dadfarnia, P. Sofronis, T. Neeraj: International Journal of Hydrogen Energy, 36
(2011) 10141–10148. J. Zhao, Z. Jiang, C. S. Lee: Corrosion Science, 82 (2014) 380–391. J. J. Au, H. K. Birnbaum: Acta Metallurgica, 26 (1978) 1105–1116. K. S. Forcey, I. Iordanova, D. K. Ross: Materials Science and Technology, 6 (1990)
357–363. R. Valentini, A. Solina: Materials Science and Technology, 10 (1994) 908–914. H. Hagi, Y. Hayashi: Trans. JIM, 28 (1987) 375–382. J. Chene, J. O. Garcia, C. P. de Oliveira, M. Aucouturier, P. Lacombe: Journal de
Microscopie et de Spectroscopie Electroniques, 4 (1979) 37–50. S. M. Myers, S. T. Picraux, R. E. Stoltz: Journal of Applied Physics, 50 (1979)
5710–5719. K. B. Kim, S. I. Pyun: Arch. Eisenhuttenwesen, 53 (1982) 397–401.
 K. T. Kim, S. L. Pyun, E. M. Riecke: Journal of Materials Science Letters, 4 (1985)624–626.
 A. T. Paxton: Materials Science and Technology, 30 (2014) 1063–1070. A. I. Shirley, C. K. Hall: Scripta Metallurgica, 17 (1983) 1003–1008. E. J. Song, H. K. D. H. Bhadeshia, D. W. Suh: Scripta Materialia, 87 (2014) 9–12. I. M. Bernstein: Scripta Materialia, 8 (1974) 343–349. A. Turnbull, R. B. Hutchings: Materials Science & Engineering A, 177 (1994) 161–
171. H. Hagi, Y. Hayashi: Trans. JIM, 28 (1987) 368–374. K. Takai, Y. Homma, K. Izutsu, M. Nagumo: Journal of the Japan Institute of
Metals, 60 (1996) 1155–1162. W. Y. Choo, J. Y. Lee: Metallurgical Transactions A, 13 (1982) 135–140. A. J. Kumnick, H. H. Johnson: Acta Metallurgica, 28 (1980) 33–39. J. L. Lee, J. Y. Lee: Metal Science, 17 (1983) 426–432. G. W. Hong, J. Y. Lee: Journal of Materials Science, 18 (1983) 271–277. F. G. Wei, T. Hara, K. Tsuzaki: Metallurgical & Materials Transactions B, 35 (2004)
587–597. F. G. Wei, K. Tsuzaki: Metallurgical & Materials Transactions A, 37 (2006) 331–
353. D. Perez Escobar, L. Duprez, A. Atrens, K. Verbeken: Materials Science and Tech-
nology, 29 (2013) 261–267. H. Asahi, D. Hirakami, S. Yamasaki: ISIJ International, 43 (2003) 527–533. D. Li, R. P. Gangloff, J. R. Scully: Metallurgical & Materials Transactions A, 35
(2004) 849–864. K. Y. Lee, J. Y. Lee, D. R. Kim: Materials Science and Engineering, 67 (1984)
213–220. I. Maroef, D. L. Olson: Weld metal hydrogen trapping: in: Joining of Advanced
Specialty Materials II: ASM International, Ohio, USA, 1999: pp. 227–235. J. L.Lee, J. Y. Lee: Metallurgical Transactions A, 17 (1986) 2183–2186. L. Remy, A. Pineau: Materials Science and Engineering, 28 (1977) 99–107. G. Frommeyer, U. Brux, P. Neumann: ISIJ International, 43 (2003) 438–446. O. Bouaziz, O. S. Allain, C. Scott: Scripta Materialia, 58 (2008) 484–487. J. K. Jung, O. Y. Lee, Y. K. Park, D. E. Kim, K. G. Jin: Korean Journal of
Materials Research, 18 (2008) 394–399. K. H. So, J. S. Kim, Y. S. Chun, K. T. Park, Y. K. Lee, C. S. Lee: ISIJ International,
49 (2009) 1952–1959. J. A. Ronevich, S. K. Kim, J. G. Speer, D. K. Matlock: Scripta Materialia, 66 (2012)
956–959. K. G. Chin, C. Y. Kang, S. Y. Shin, S. K. Hong, S. H. Lee, H. S. Kim, K. H. Kim,
N. J. Kim: Materials Science & Engineering A, 528 (2011) 2922–2928. M. Koyama, E. Akiyama, T. Sawaguchi, D. Raabe, K. Tsuzaki: Scripta Materialia,
66 (2012) 459–462. P. Lan, L. Song, C. Du, J. Zhang: Materials Science and Technology, 30 (2014)
 H.-J. Kim, S.-K. Youn: Journal of Manufacturing Science and Engineering, Trans-actions of the ASME, 130 (2008) 0310051–0310057.
 M. Koyama, E. Akiyama, K. Tsuzak: ISIJ international, 53 (2013) 1268–1274. I. Park, K. Jeong, J. Jung, C. Lee, Y. Lee: Int J Hydrogen Energy, 37 (2012)
9925–9932. Y. Chun, K. Park, C. Lee: Scripta Mater, 66 (2012) 960–965. J. H. Ryu, S. K. Kim, C. S. Lee, D. W. Suh, H. K. D. H. Bhadeshia: Proceedings of
the Royal Society A, 469 (2013) 20120458. D. K. Han, Y. Kim, H. N. Han, H. K. D. H. Bhadeshia, D. W. Suh: Scripta Mate-
rialia, 80 (2014) 9–12. Y. Li, C. Chen, F. Zhang: Advances in Materials Science and Engineering, 2013
(2013) 382060. S. Fukui: Testu to Hagane, 55 (1969) 151–161. E. C. Bain: Alloying Elements in Steel: American Society of Materials, Cleveland,
Ohio, USA, 1939. A. G. Allten, P. Payson: Trans. ASM, 45 (1953) 498–532. W. S. Owen: Trans. ASM, 46 (1954) 812–829. A. S. Keh: Acta Metallurgica, 11 (1963) 1101–1103. J. Gordine, I. Codd: Journal of the Iron and Steel Institute, 207 (1969) 461–467. R. M. Hobbs, G. W. Lorimer, N. Ridley: Journal of the Iron and Steel Institute,
210 (1972) 757–764. W. J. Nam: ISIJ International, 39 (1999) 1181–1187. E. Kozeschnik, H. K. D. H. Bhadeshia: Materials Science and Technology, 24 (2008)
343–347. J. H. Jang, I. G. Kim, H. K. D. H. Bhadeshia: Computational Materials Science, 44
(2009) 1319–1326. J. H. Jang, I. G. Kim, H. K. D. H. Bhadeshia: Materials Science Forum, 638-642
(2010) 3319–3324. G. Miyamoto, J. C. Oh, K. Hono, T. Furuhara, T. Maki: Acta Materialia, 55 (2007)
5027–5038. B. D. Craig: Acta Metallurgica, 25 (1977) 1027–1030. F. G. Wei, K. Tsuzaki: Scripta Materialia, 52 (2005) 467–472. F. G. Wei, T. Hara, T. Tsuchida, K. Tsuzaki: ISIJ International, 43 (2003) 539–547. M. F. Stevens, I. M. Bernstein: Metallurgical Transactions A, 20 (1989) 909–919. T. G. Owe Berg: The effect of ε-carbide on the passivity of steel in nitric acid
solutions: Tech. Rep. 1310-62(02)SP, Appendix C: Aerojet-General Corporation,Ordnance Division: California, USA (1962).
 X. Zhu, W. Li, T. Y. Hsu, S. Zhou, L. Wang, X. Jin: Scripta Materialia, 97 (2015)21–24.
 K. Kawakami, T. Matsumiya: ISIJ International, 52 (2012) 1693–1697. H. K. D. H. Bhadeshia: Bainite in steels: theory and practice: 3rd Edition: Maney
Publishing, Leeds, U.K., 2015. S. Yamasaki, H. K. D. H. Bhadeshia: Materials Science and Technology, 19 (2003)
 S. Yamasaki, H. K. D. H. Bhadeshia: Proceedings of the Royal Society of London A,462 (2006) 2315–2330.
 R. K. W. Marceau: Materials Science and Technology, 31 (2015) DOI10.1179/1743284715Y.0000000088.
 J. Takahashi, K. Kawakami, T. Tarui: Scripta Materialia, 67 (2012) 213–216. T. Kushida, N. Kuratomi, T. Kudoh, H. Matsumoto, T. Tsumura, F. Nakasato:
Tetsu-to-Hagane, 82 (1996) 297–302. Y. Kimura, T. Hara, K. Tsuzaki: CAMP-ISIJ, 14 (2001) 1307. S. Li, E. Akyama, K. Yuuji, K. Tsuzaki, N. Uno, B. Zhang: Science and Technology
of Advanced Materials, 11 (2010) 025005. E. Akiyama: ISIJ International, 52 (2012) 307–315. S. Matera, E. Anelli: Microscopy Microanalysis Microstructures, 6 (1995) 633–646. J. A. Spitzangel, S. S. Brenner, M. K. Miller, W. J. Choyke: Journal of Nuclear
Materials, 122-123 (1984) 252–253. J. Takahashi, K. Kawakami, Y. Kobayashi, T. Tarui: Scripta Materialia, 63 (2010)
261–264. Y. Matsubara, H. Hamada: A novel method to evaluate the influence of hydrogen
on fatigue properties of high strength steels: in: J. M. Beswick (Ed.), Bearing SteelTechnology – Advances and State of the Art in Bearing Steel Quality Assurance:ASTM International, West Conshohocken, PA, USA, 2007: pp. 153–166.
 H. K. D. H. Bhadeshia: Progress in Materials Science, 57 (2012) 268–435. Y. Furuya, H. Hirukawa, M. Hayakawa: Metallurgical & Materials Transactions A,
41 (2010) 2248–2256. M. Nagumo, K. Takai, N. Okuda: Journal of Alloys and Compounds, 293-295 (1999)
310–316. M. Aoki, H. Saito, M. Mori, Y. Ishida, M. Nagumo: Journal of the Japan Institute
of Metals, 58 (1994) 1141–1148. S. Suzuki, N. Ishii, T. Miyagawa, H. Harada: Tetsu-to-Hagane, 79 (1993) 227–232. T. Tarui, S. Yamasaki: Tetsu-to-Hagane, 88 (2012) 612–619. S. Suzuki, G. Rees, H. K. D. H. Bhadeshia: Modelling of brittle zones in the HAZ
of steel welds: in: T. Zacharia (Ed.), Modelling and Control of Joining Processes,:American Welding Society, Florida, USA, 1993: pp. 186–193.
 G. Mansilla, S. Herenu, E. Brandaleze: Materials Science and Technology, 30 (2013)501–505.
 T. Karsch, H. Bomas, H. W. Zoch, S. Mandl: International Journal of Fatigue, 60(2014) 74–89.
 H. K. D. H. Bhadeshia, W. Solano-Alvarez: Machining Science and Technology, 31(2015) 1011–1105.
 Y. D. Park, I. S. Maroef, A. Landau, D. L. Olson: Welding Journal, ResearchSupplement, 81 (2002) 27S–35S.
 J. L. Gu, K. D. Chang, H. S. Fang, Z. G. Yang, B. Z. Bai: Journal of Iron and SteelResearch, International, 11 (2004) 42–46.
 T. Hojo, S. M. Song, K. Sugimoto, Y. Mukai, S. Ikeda: Hydrogen embrittlementof ultra high strength low alloy TRIP-aided steel: in: 2nd Int. Conf. on AdvancedStructural Steels: Chinese Society for Metals, Beijing, China, 2004: pp. 638–641.
 T. Hojo, S. M. Song, K. Sugimoto, A. Nagasaka, S. Ikeda, H. Akamizu,M. Mayuzumi: Tetsu-to-Hagane, 90 (2004) 65–69.
 K. I. Sugimoto: Materials Science and Technology, 25 (2009) 1108–1117. H. Tsubakino, H. Harada, J. Yin: ISIJ International, 39 (1999) 298–300. M. Wang, C. C. Tasan, M. Koyama, D. Ponge, D. Raabe: Metallurgical & Materials
Transactions A, 46 (2015) 3797–3802. L. C. D. Fielding, E. J. Song, D. K. Han, H. K. D. H. Bhadeshia, D. W. Suh:
Proceedings of the Royal Society of London A, 470 (2014) 20140108. E. Skolek, S. Marciniak, P. Skoczylas, J. Kaminski, W. Swiatnicki: Archives of
Metallurgy and Materials, 60 (2015) 491–496. K. J. L. Iyer: Materials Science & Engineering, 100 (1988) L7–L8. G. T. Park, S. U. Koh, H. G. Jung, K. Y. Kim: Corrosion Science, 50 (2008)
1865–1871. H. Ma, Z. Liu, C. Du, H. Wang, X. Li: Materials Science & Engineering A, 642